Standard Specification for Low-Alloy Steel Deformed and Plain Bars for Concrete Reinforcement
This specification covers deformed and plain low-alloy steel bars in cut lengths or coils for concrete reinforcement intended for applications. Restrictive mechanical properties and chemical composition are required for compatibility with controlled tensile property applications or to enhance weldability. The steel shall be electric-furnace, basic-oxygen, or open-hearth processed. Tension test, bend test, and one set of dimensional property tests including bar weight and spacing, height, and gap of deformations shall be made of each bar size rolled from a heat. All tests and inspection shall be made at the place of manufacture prior to shipment, unless otherwise specified, and shall be conducted so as not to interfere unnecessarily with the operation of the works. A retest shall be provided when the specimen fails to meet the strength and elongation property requirements of the specification.
1.1 General—This specification covers deformed and plain low-alloy steel bars in cut lengths or coils for concrete reinforcement intended for applications where restrictive mechanical properties and chemical composition are required for compatibility with controlled tensile property applications or to enhance weldability. The standard sizes and dimensions of deformed bars and their number designations are given in Table 1. The text of this specification references notes and footnotes that provide explanatory material. These notes and footnotes, excluding those in tables, shall not be considered as requirements of this specification.
1.2 Grade—Bars are of two minimum yield strength levels: namely, 60 000 psi [420 MPa] and 80 000 , designated as Grade 60  and Grade 80 , respectively.
1.3 Plain bars, in sizes up to and including 21/2 in. [63.5 mm] in diameter in coils or cut lengths, when ordered, shall be furnished under this specification. For ductility properties (elongation and bending), test provisions of the nearest smaller nominal diameter deformed bar size shall apply.
1.4 Controlled Tensile Properties—This specification limits mechanical properties (Table 2) to provide the desired yield/tensile properties for controlled tensile property applications.
1.5 Welding—This specification limits chemical composition (6.2) and carbon equivalent (6.4) to enhance the weldability of the material. When steel is to be welded, a welding procedure suitable for the chemical composition and intended use or service should be used. The use of the latest edition of AWS D1.4/D1.4M is recommended. This document describes the proper selection of the filler metals, preheat/interpass temperatures, as well as, performance and procedure qualification requirements.
1.6 Requirements for alternate bar sizes are presented in Annex A1. The requirements in Annex A1 only apply when specified by the purchaser (see 4.1.9).
1.7 This specification is applicable for orders in either inch-pound units (Specification A706) or in SI units [Specification A706M].
1.8 The values stated in either inch-pound units or SI units are to be regarded as standard. Within the text, the SI units are shown in brackets. The values stated in each system are not exact equivalents; therefore, each system must be used independently of the other. Combining values from the two systems may result in nonconformance with this specification.
1.9 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
Formato físico y digital
Nota: Precios sin IVA ni gastos de envío
Añadir a la cesta